Nanoclay addition to a conventional glass ionomer cements: Influence on physical properties
Objective: The objective of the present study is to investigate the reinforcement effect of  polymer-grade montmorillonite (PGN nanoclay) on physical properties of glass ionomer cement (GIC). Materials and Methods: The PGN nanoclay was dispersed in the liquid portion of GIC (HiFi, Advanced Healthcare, Kent, UK) at 1%, 2% and 4% (w/w). Fourier-transform infrared (FTIR) spectroscopy was used to quantify the polymer liquid of GICs after dispersion of nanoclay. The molecular weight (M w ) of HiFi liquid was determined by gel permeation chromatography. The compressive strength (CS), diametral-tensile strength, flexural strength (FS) and flexural modulus (E f ) of cements (n = 20) were measured after storage for 1 day, 1 week and 1 month. Fractured surface was analyzed by scanning electron microscopy. The working and setting time (WT and ST) of cements was measured by a modified Wilson′s rheometer. Results: The FTIR results showed a new peak at 1041 cm−1 which increased in intensity with an increase in the nanoclay content and was related to the Si-O stretching mode in PGN nanoclay. The M w of poly (acrylic acid) used to form cement was in the range of 53,000 g/mol. The nanoclay reinforced GICs containing <2% nanoclays exhibited higher CS and FS. The E f cement with 1% nanoclays was significantly higher. The WT and ST of 1% nanoclay reinforced cement were similar to the control cement but were reduced with 2% and 4% nanoclay addition. Conclusion: The dispersion of nanoclays in GICs was achieved, and GIC containing 2 wt% nanoclay is a promising restorative materials with improved physical properties.
Maturation processes in glass-ionomer dental cements
Abstract Glass-ionomer cements are used for a variety of tooth-repair functions in clinical dentistry. They are formed by reaction of a basic glass powder with a solution of polymeric water-soluble acid, usually polyacrylic acid. After the initial neutralization reaction, by which the cement hardens, various maturation reactions occur. Changes induced by these maturation reactions are identified as: increase in strength; reduction in plasticity; improvement in opacity; and increase in proportion of tightly bound water. In addition, in contact with the tooth, an ion-exchange interfacial layer is gradually formed. This is mechanically strong and chemically-resistant. These changes are described in the current paper, which reviews the extent to which they occur, and reports what is know about the chemistry that underlies them. Processes involving slow diffusion of various ions and of water through the set cement bring about these changes. They include a secondary setting reaction to form a phosphate-based phase, binding of water to co-ordination sites around metal cations and to a hydration sheath around the polymer molecules, and possibly reaction of water with glass particle surfaces to form silanol groups. Evidence from a wide range of literature sources is used to be build up a detailed picture of the chemistry of the maturation processes, and gaps in our understanding are highlighted. The article concludes that, given the importance of glass-ionomers in contemporary dentistry, it is important to know the extent to which such maturation processes occur in current cement formulations, and also to determine how rapidly they take place.
Hygroscopic Expansion of some Casting Investments
CREDIT is generally given to Taggart1 for introducing the cast gold inlay to the dental profession. Although he realized that gold shrinks when cooled from molten state to solid state of room temperature, the investment available to him did not supply sufficient compensation. In 1910, Van Horn2 published a paper dealing with a method by which he obtained the compensation by means of wax expansion. The next major research in connection with this problem was the work of Coleman3 at the National Bureau of Standards. He determined the gold shrinkage to be 1.25 per cent and presented a casting technic with compensation values of quantitative nature. The total compensation for the gold shrinkage was obtained by the combination of the setting and thermal expansion of the mold. This procedure is the general practice followed at the present time for compensation. There are some disadvantages to this method. Skinner has indicated the difficulty of obtaining smooth castings and the improper compensation for the casting shrinkage.4 It has been found by Hollenback5 and Scheu6a that castings made at a high temperature are rougher than those made at a low temperature (450° C.), depending upon the great difference in thermal expansion between plaster of Paris and silica, which causes a poor union of the fine particles. This may also result in friability and there may be some warpage due to the differential expansion. A method which provides sufficient compensation at a low mold temperature is the hygroscopic casting technic.b Wilson7 showed that certain plasters expand as much as 0.0044 inch to the inch by taking up moisture from the air. With this information at hand, Scheula, b tested some commercial investment to determine what results the addition of moisture would have. He found6b: (1) All of the casting investments that were tested expanded. (2) The thicker the mix, the greater the expansion. (3) A mix with hot water expanded more than one with cold water. (4) The time at which the mix is placed in the water is of great importance. It was found that if the mix is placed in the water early, it would not expand so much as when placed in a little later. It was also found that if the mix was placed in the water after a certain time, it could not expand to the maximal amount. (5) The temperature of the water in which the mix is placed is important, for two reasons; (a) the temperature of the water controls slightly the expansion of the investment, and (b) water at a temperature of 1000 F. slightly softens the wax pattern so that the fine margins are not marred while expansion is taking place. The mix should remain in the water at least 20 minutes to obtain the full expansion, after which time no further expansion is obtained.